#------------------------------------------------------------------------------
#$Date: 2016-02-20 05:06:23 +0200 (Sat, 20 Feb 2016) $
#$Revision: 176774 $
#$URL: svn://www.crystallography.net/cod/cif/2/20/23/2202379.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2202379
loop_
_publ_author_name
'Yang, Shi-Yao'
'Long, La-Sheng'
'Huang, Rong-Bin'
'Zheng, Lan-Sun'
'Ng, Seik Weng'
_publ_section_title
;
 On the number of uncoordinated water molecules in the open-framework
 coordination compound,
 bis(1,2,4,5-benzenetetracarboxylato)dihydroxytetraaquapentacobalt(II)
 x-hydrate, and the crystal structure of the isomorphous
 decahydrated zinc(II) analog
;
_journal_issue                   10
_journal_name_full               'Acta Crystallographica Section E'
_journal_page_first              m921
_journal_page_last               m923
_journal_paper_doi               10.1107/S1600536803019895
_journal_volume                  59
_journal_year                    2003
_chemical_formula_iupac          '[Zn5 (OH)2 (C10 H2 O8)2 (H2 O)4].10(H2 O)'
_chemical_formula_moiety         '[Zn5 (OH)2 (C10 H2 O8)2 (H2 O)4], 10(H2 O)'
_chemical_formula_sum            'C20 H34 O32 Zn5'
_chemical_formula_weight         1113.32
_chemical_name_systematic
;
 Bis(1,2,4,5-benzenetetracarboxylato)dihydroxytetraaquapentazinc(II)
 decahydrate
;
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2yn'
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90
_cell_angle_beta                 94.9930(10)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   7.4087(3)
_cell_length_b                   16.4236(6)
_cell_length_c                   14.5347(5)
_cell_measurement_reflns_used    9591
_cell_measurement_temperature    298(2)
_cell_measurement_theta_max      28.3
_cell_measurement_theta_min      2.5
_cell_volume                     1761.84(11)
_computing_cell_refinement       'SAINT (Bruker, 2001)'
_computing_data_collection       'SMART (Bruker, 2001)'
_computing_data_reduction        'SAINT (Bruker, 2001)'
_computing_molecular_graphics    'ORTEPII (Johnson, 1976)'
_computing_publication_material  'SHELXL97 (Sheldrick, 1997)'
_computing_structure_refinement  'SHELXL97 (Sheldrick, 1997)'
_diffrn_ambient_temperature      298(2)
_diffrn_measured_fraction_theta_full 1.00
_diffrn_measured_fraction_theta_max 1.00
_diffrn_measurement_device_type
'Bruker APEX CCD area-detector diffractometer'
_diffrn_measurement_method       'φ and ω scan'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.048
_diffrn_reflns_av_sigmaI/netI    0.034
_diffrn_reflns_limit_h_max       8
_diffrn_reflns_limit_h_min       -8
_diffrn_reflns_limit_k_max       19
_diffrn_reflns_limit_k_min       -19
_diffrn_reflns_limit_l_max       17
_diffrn_reflns_limit_l_min       -17
_diffrn_reflns_number            16789
_diffrn_reflns_theta_full        25.0
_diffrn_reflns_theta_max         25.0
_diffrn_reflns_theta_min         1.9
_diffrn_standards_decay_%        0
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    3.47
_exptl_absorpt_correction_T_max  0.708
_exptl_absorpt_correction_T_min  0.585
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS (Sheldrick, 1996)'
_exptl_crystal_colour            Colorless
_exptl_crystal_density_diffrn    2.099
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       Parallelepiped
_exptl_crystal_F_000             1120
_exptl_crystal_size_max          0.20
_exptl_crystal_size_mid          0.14
_exptl_crystal_size_min          0.10
_refine_diff_density_max         0.69
_refine_diff_density_min         -0.73
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.27
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     259
_refine_ls_number_reflns         3105
_refine_ls_number_restraints     30
_refine_ls_restrained_S_all      1.27
_refine_ls_R_factor_all          0.063
_refine_ls_R_factor_gt           0.062
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         <0.001
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w = 1/[σ²(Fo²)+(0.0317P)²+13.7636P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.129
_refine_ls_wR_factor_ref         0.129
_reflns_number_gt                3079
_reflns_number_total             3105
_reflns_threshold_expression     I>2σ(I)
_cod_data_source_file            bt6349.cif
_cod_data_source_block           I
_cod_depositor_comments
;
The following automatic conversions were performed:
'_symmetry_cell_setting' value 'Monoclinic' changed to 'monoclinic'
according to '/home/saulius/struct/CIF-dictionaries/cif_core.dic'
dictionary named 'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_enum 1527 2010-12-29 10:47:43Z saulius 

The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Monoclinic' changed to 'monoclinic'
according to /home/saulius/struct/CIF-dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.1 from
2010-06-29.

'_exptl_absorpt_correction_type' value 'Multi-scan'
changed to 'multi-scan' according to
/home/saulius/struct/CIF-dictionaries/cif_core.dic dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_values 1715 2011-07-08 13:25:40Z adriana 
;
_cod_original_cell_volume        1761.80(10)
_cod_original_sg_symbol_H-M      'P 21/n'
_cod_database_code               2202379
_cod_database_fobs_code          2202379
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x-1/2, -y-1/2, z-1/2'
loop_
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
_atom_site_type_symbol
Zn1 0.5000 0.5000 0.5000 0.0151(2) Uani d S 1 . . Zn
Zn2 0.22160(10) 0.48192(5) 0.68087(5) 0.0212(2) Uani d . 1 . . Zn
Zn3 0.80870(10) 0.62723(5) 0.52090(5) 0.0206(2) Uani d . 1 . . Zn
O1 0.5300(7) 0.8410(3) 0.9574(3) 0.0320(10) Uani d . 1 . . O
O2 0.4826(7) 0.8947(3) 0.8167(3) 0.0290(10) Uani d . 1 . . O
O3 1.1222(6) 0.8138(3) 0.9397(4) 0.0370(10) Uani d . 1 . . O
O4 0.8962(6) 0.9041(3) 0.9191(3) 0.0250(10) Uani d . 1 . . O
O5 0.9763(6) 0.5870(3) 0.6284(3) 0.0270(10) Uani d . 1 . . O
O6 1.0728(6) 0.5496(3) 0.7671(3) 0.0230(10) Uani d . 1 . . O
O7 0.4217(7) 0.5705(4) 0.7169(4) 0.0400(10) Uani d . 1 . . O
O8 0.5986(6) 0.5843(3) 0.6027(3) 0.0220(10) Uani d . 1 . . O
O9 0.2460(6) 0.4826(3) 0.5465(3) 0.0180(10) Uani d . 1 . . O
O1w 0.8420(10) 0.7587(5) 0.5717(5) 0.073(2) Uani d . 1 . . O
O2w 0.3799(8) 0.4070(3) 0.7644(4) 0.0440(10) Uani d . 1 . . O
O3w 0.7530(10) 0.9253(5) 0.6824(5) 0.076(2) Uani d U 1 . . O
O4w 0.142(2) 0.0994(7) 0.5710(7) 0.119(4) Uani d U 1 . . O
O5w 0.219(2) 0.7697(8) 0.6310(10) 0.144(4) Uani d U 1 . . O
O6w 0.775(2) 0.0433(9) 0.5430(10) 0.159(5) Uani d U 1 . . O
O7w 0.491(2) 0.8410(10) 0.5490(10) 0.192(6) Uani d U 1 . . O
C1 0.6693(8) 0.7803(4) 0.8356(4) 0.0170(10) Uani d . 1 . . C
C2 0.8569(9) 0.7747(4) 0.8524(4) 0.0190(10) Uani d . 1 . . C
C3 0.9465(8) 0.7105(4) 0.8128(4) 0.0200(10) Uani d . 1 . . C
C4 0.8561(8) 0.6545(4) 0.7552(4) 0.0160(10) Uani d . 1 . . C
C5 0.6673(8) 0.6597(4) 0.7401(4) 0.0170(10) Uani d . 1 . . C
C6 0.5770(8) 0.7216(4) 0.7805(4) 0.0190(10) Uani d . 1 . . C
C7 0.5541(8) 0.8457(4) 0.8741(5) 0.0210(10) Uani d . 1 . . C
C8 0.9656(9) 0.8363(4) 0.9080(4) 0.0210(10) Uani d . 1 . . C
C9 0.9719(8) 0.5921(4) 0.7137(4) 0.0190(10) Uani d . 1 . . C
C10 0.5544(9) 0.5993(4) 0.6810(4) 0.0200(10) Uani d . 1 . . C
H9 0.1638 0.5240 0.5180 0.021 Uiso calc R 1 . . H
H1w1 0.7807 0.7975 0.5446 0.050 Uiso d . 1 . . H
H1w2 0.9281 0.7789 0.6069 0.050 Uiso d . 1 . . H
H2w1 0.3648 0.3578 0.7809 0.050 Uiso d . 1 . . H
H2w2 0.3587 0.4387 0.8082 0.050 Uiso d . 1 . . H
H3w1 0.6984 0.9477 0.7250 0.050 Uiso d . 1 . . H
H3w2 0.7742 0.9611 0.6421 0.050 Uiso d . 1 . . H
H4w1 0.2347 0.0756 0.5528 0.050 Uiso d . 1 . . H
H4w2 0.0574 0.0636 0.5744 0.050 Uiso d . 1 . . H
H5w1 0.2518 0.7269 0.6015 0.050 Uiso d . 1 . . H
H5w2 0.2106 0.8089 0.5898 0.050 Uiso d . 1 . . H
H6w1 0.6645 0.0254 0.5282 0.050 Uiso d . 1 . . H
H6w2 0.7988 0.0748 0.4971 0.050 Uiso d . 1 . . H
H7w1 0.5163 0.8767 0.5065 0.050 Uiso d . 1 . . H
H7w2 0.5243 0.8649 0.6015 0.050 Uiso d . 1 . . H
H3 1.0712 0.7054 0.8258 0.024 Uiso calc R 1 . . H
H6 0.4514 0.7244 0.7708 0.023 Uiso calc R 1 . . H
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Zn Zn 0.2839 1.4301 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle
_geom_angle_publ_flag
O4 Zn1 O4 2_646 4_575 180.0(2) yes
O4 Zn1 O8 2_646 . 90.5(2) yes
O4 Zn1 O8 2_646 3_666 89.5(2) yes
O4 Zn1 O9 2_646 . 90.8(2) yes
O4 Zn1 O9 2_646 3_666 89.3(2) yes
O4 Zn1 O8 4_575 . 89.5(2) no
O4 Zn1 O8 4_575 3_666 90.5(2) no
O4 Zn1 O9 4_575 . 89.3(2) no
O4 Zn1 O9 4_575 3_666 90.8(2) no
O8 Zn1 O8 . 3_666 180.0(2) yes
O8 Zn1 O9 . . 97.3(2) yes
O8 Zn1 O9 . 3_666 82.7(2) yes
O8 Zn1 O9 3_666 . 82.7(2) no
O8 Zn1 O9 3_666 3_666 97.3(2) no
O9 Zn1 O9 . 3_666 180.0 yes
O2 Zn2 O5 2_546 1_455 88.4(2) yes
O2 Zn2 O6 2_546 1_455 86.2(2) yes
O2 Zn2 O7 2_546 . 164.6(2) yes
O2 Zn2 O9 2_546 . 98.6(2) yes
O2 Zn2 O2w 2_546 . 87.5(2) yes
O5 Zn2 O6 1_455 1_455 54.42(16) yes
O5 Zn2 O7 1_455 . 94.2(2) yes
O5 Zn2 O9 1_455 . 80.0(2) yes
O5 Zn2 O2w 1_455 . 160.2(2) yes
O6 Zn2 O7 1_455 . 83.04(19) yes
O6 Zn2 O9 1_455 . 134.1(2) yes
O6 Zn2 O2w 1_455 . 105.9(2) yes
O7 Zn2 O9 . . 96.8(2) yes
O7 Zn2 O2w . . 85.0(2) yes
O9 Zn2 O2w . . 119.8(2) yes
O1 Zn3 O3 4_675 4_575 98.8(2) yes
O1 Zn3 O5 4_675 . 88.2(2) yes
O1 Zn3 O8 4_675 . 171.8(2) yes
O1 Zn3 O9 4_675 3_666 98.2(2) yes
O1 Zn3 O1w 4_675 . 80.5(3) yes
O3 Zn3 O5 4_575 . 165.2(2) yes
O3 Zn3 O8 4_575 . 89.4(2) yes
O3 Zn3 O9 4_575 3_666 92.7(2) yes
O3 Zn3 O1w 4_575 . 77.4(2) yes
O5 Zn3 O8 . . 83.8(2) yes
O5 Zn3 O9 . 3_666 99.3(2) yes
O5 Zn3 O1w . . 91.0(2) yes
O8 Zn3 O9 . 3_666 81.7(2) yes
O8 Zn3 O1w . . 101.1(2) yes
O9 Zn3 O1w 3_666 . 169.5(2) yes
C7 O1 Zn3 . 4_576 128.4(4) no
C7 O2 Zn2 . 2_556 134.4(4) no
C8 O3 Zn3 . 4_676 129.9(4) no
C8 O4 Zn1 . 2_656 128.1(4) no
C9 O5 Zn3 . . 132.8(4) no
C9 O6 Zn2 . 1_655 104.3(4) no
C10 O7 Zn2 . . 136.1(4) no
C10 O8 Zn1 . . 132.6(4) no
C10 O8 Zn3 . . 134.7(4) no
Zn1 O8 Zn3 . . 92.7(2) no
Zn2 O9 Zn1 . . 119.1(2) no
Zn2 O9 Zn3 . 3_666 115.5(2) no
Zn1 O9 Zn3 . 3_666 96.4(2) no
C2 C1 C6 . . 119.1(6) no
C2 C1 C7 . . 124.8(6) no
C6 C1 C7 . . 116.1(5) no
C1 C2 C3 . . 118.8(6) no
C1 C2 C8 . . 122.3(6) no
C3 C2 C8 . . 118.9(6) no
C4 C3 C2 . . 122.1(6) no
C3 C4 C5 . . 118.7(6) no
C3 C4 C9 . . 115.9(5) no
C5 C4 C9 . . 125.4(5) no
C6 C5 C4 . . 119.7(6) no
C6 C5 C10 . . 117.4(5) no
C4 C5 C10 . . 122.9(5) no
C5 C6 C1 . . 121.6(6) no
O1 C7 O2 . . 127.3(6) no
O1 C7 C1 . . 116.8(6) no
O2 C7 C1 . . 115.7(6) no
O4 C8 O3 . . 126.2(6) no
O4 C8 C2 . . 118.0(6) no
O3 C8 C2 . . 115.8(6) no
O5 C9 O6 . . 121.1(6) no
O5 C9 C4 . . 120.9(6) no
O6 C9 C4 . . 117.8(6) no
O8 C10 O7 . . 126.3(6) no
O8 C10 C5 . . 118.3(6) no
O7 C10 C5 . . 115.3(5) no
Zn2 O9 H9 . . 108.3 no
Zn1 O9 H9 . . 108.3 no
Zn3 O9 H9 3_666 . 108.3 no
Zn3 O1w H1w1 . . 121 no
Zn3 O1w H1w2 . . 128 no
H1w1 O1w H1w2 . . 109 no
Zn2 O2w H2w1 . . 131 no
Zn2 O2w H2w2 . . 87 no
H2w1 O2w H2w2 . . 109 no
H3w1 O3w H3w2 . . 109 no
H4w1 O4w H4w2 . . 108 no
H5w1 O5w H5w2 . . 106 no
H6w1 O6w H6w2 . . 106 no
H7w1 O7w H7w2 . . 104 no
C4 C3 H3 . . 119.0 no
C2 C3 H3 . . 119.0 no
C5 C6 H6 . . 119.2 no
C1 C6 H6 . . 119.2 no
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_2
_geom_bond_distance
_geom_bond_publ_flag
Zn1 O4 2_646 2.072(4) yes
Zn1 O4 4_575 2.072(4) no
Zn1 O9 . 2.074(4) yes
Zn1 O9 3_666 2.074(4) no
Zn1 O8 . 2.119(4) yes
Zn1 O8 3_666 2.119(4) no
Zn2 O2 2_546 2.086(5) yes
Zn2 O5 1_455 2.573(5) yes
Zn2 O6 1_455 2.064(4) yes
Zn2 O7 . 2.111(5) yes
Zn2 O9 . 1.977(4) yes
Zn2 O2w . 2.029(6) yes
Zn3 O1 4_675 2.019(5) yes
Zn3 O3 4_575 1.990(5) yes
Zn3 O5 . 2.021(5) yes
Zn3 O8 . 2.158(4) yes
Zn3 O9 3_666 2.076(4) yes
Zn3 O1w . 2.288(8) yes
O1 C7 . 1.241(8) no
O2 C7 . 1.244(8) no
O3 C8 . 1.265(8) no
O4 C8 . 1.244(8) no
O5 C9 . 1.245(8) no
O6 C9 . 1.245(8) no
O7 C10 . 1.246(8) no
O8 C10 . 1.236(8) no
C1 C2 . 1.393(9) no
C1 C6 . 1.394(9) no
C1 C7 . 1.509(9) no
C2 C3 . 1.396(9) no
C2 C8 . 1.487(9) no
C3 C4 . 1.378(9) no
C4 C5 . 1.400(9) no
C4 C9 . 1.496(9) no
C5 C6 . 1.376(9) no
C5 C10 . 1.516(9) no
O9 H9 . 0.98 no
O1w H1w1 . 0.86 no
O1w H1w2 . 0.85 no
O2w H2w1 . 0.85 no
O2w H2w2 . 0.85 no
O3w H3w1 . 0.85 no
O3w H3w2 . 0.86 no
O4w H4w1 . 0.86 no
O4w H4w2 . 0.86 no
O5w H5w1 . 0.87 no
O5w H5w2 . 0.88 no
O6w H6w1 . 0.88 no
O6w H6w2 . 0.87 no
O7w H7w1 . 0.89 no
O7w H7w2 . 0.87 no
C3 H3 . 0.93 no
C6 H6 . 0.93 no
loop_
_geom_hbond_atom_site_label_D
_geom_hbond_atom_site_label_H
_geom_hbond_atom_site_label_A
_geom_hbond_site_symmetry_A
_geom_hbond_distance_DH
_geom_hbond_distance_HA
_geom_hbond_distance_DA
_geom_hbond_angle_DHA
_geom_hbond_publ_flag
O9 H9 O5 1_455 0.98 2.44 2.960(10) 113 yes
O1w H1w2 O5w 1_655 0.85 2.16 2.86(2) 139 yes
O1w H1w1 O7w . 0.86 2.27 2.92(2) 133 yes
O2w H2w1 O5w 2_546 0.85 2.06 2.85(2) 153 yes
O3w H3w1 O2 . 0.85 2.34 2.960(10) 130 yes
O3w H3w2 O6w 1_565 0.86 1.98 2.82(2) 169 yes
O4w H4w1 O6w 3_656 0.86 2.39 2.96(2) 125 yes
O4w H4w2 O6w 1_455 0.86 2.13 2.87(2) 143 yes
O5w H5w2 O7w . 0.88 2.27 2.69(2) 110 yes
O7w H7w1 O6w 3_666 0.89 2.57 2.97(2) 108 yes
O7w H7w2 O3w . 0.87 2.21 2.96(2) 144 yes
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
_geom_torsion
_geom_torsion_publ_flag
O3 Zn3 O5 C9 4_575 . 20.0(10) no
O1 Zn3 O5 C9 4_675 . 138.7(6) no
O9 Zn3 O5 C9 3_666 . -123.3(6) no
O8 Zn3 O5 C9 . . -42.8(6) no
O1w Zn3 O5 C9 . . 58.2(6) no
O9 Zn2 O7 C10 . . -20.6(8) no
O2w Zn2 O7 C10 . . 98.9(8) no
O6 Zn2 O7 C10 1_455 . -154.3(8) no
O2 Zn2 O7 C10 2_546 . 159.8(7) no
O5 Zn2 O7 C10 1_455 . -101.0(7) no
O4 Zn1 O8 C10 4_575 . 110.9(6) no
O4 Zn1 O8 C10 2_646 . -69.1(6) no
O9 Zn1 O8 C10 3_666 . -158.3(6) no
O9 Zn1 O8 C10 . . 21.7(6) no
O4 Zn1 O8 Zn3 4_575 . -71.9(2) no
O4 Zn1 O8 Zn3 2_646 . 108.1(2) no
O9 Zn1 O8 Zn3 3_666 . 18.9(2) no
O9 Zn1 O8 Zn3 . . -161.1(2) no
O3 Zn3 O8 C10 4_575 . -109.0(6) no
O5 Zn3 O8 C10 . . 57.8(6) no
O9 Zn3 O8 C10 3_666 . 158.2(6) no
O1w Zn3 O8 C10 . . -32.0(7) no
O3 Zn3 O8 Zn1 4_575 . 73.8(2) no
O5 Zn3 O8 Zn1 . . -119.4(2) no
O9 Zn3 O8 Zn1 3_666 . -19.0(2) no
O1w Zn3 O8 Zn1 . . 150.8(2) no
O2w Zn2 O9 Zn1 . . -52.9(3) no
O6 Zn2 O9 Zn1 1_455 . 122.1(3) no
O2 Zn2 O9 Zn1 2_546 . -144.9(2) no
O7 Zn2 O9 Zn1 . . 35.2(3) no
O5 Zn2 O9 Zn1 1_455 . 128.3(2) no
O2w Zn2 O9 Zn3 . 3_666 61.0(3) no
O6 Zn2 O9 Zn3 1_455 3_666 -124.0(2) no
O2 Zn2 O9 Zn3 2_546 3_666 -31.0(3) no
O7 Zn2 O9 Zn3 . 3_666 149.1(2) no
O5 Zn2 O9 Zn3 1_455 3_666 -117.7(2) no
O4 Zn1 O9 Zn2 4_575 . -125.7(2) no
O4 Zn1 O9 Zn2 2_646 . 54.3(2) no
O8 Zn1 O9 Zn2 . . -36.3(3) no
O8 Zn1 O9 Zn2 3_666 . 143.7(3) no
O4 Zn1 O9 Zn3 4_575 3_666 110.4(2) no
O4 Zn1 O9 Zn3 2_646 3_666 -69.6(2) no
O8 Zn1 O9 Zn3 . 3_666 -160.2(2) no
O8 Zn1 O9 Zn3 3_666 3_666 19.8(2) no
C6 C1 C2 C3 . . 0.3(9) no
C7 C1 C2 C3 . . 179.5(6) no
C6 C1 C2 C8 . . 178.0(6) no
C7 C1 C2 C8 . . -3.0(10) no
C1 C2 C3 C4 . . 2.0(10) no
C8 C2 C3 C4 . . -175.4(6) no
C2 C3 C4 C5 . . -4.0(10) no
C2 C3 C4 C9 . . 176.5(6) no
C3 C4 C5 C6 . . 1.9(9) no
C9 C4 C5 C6 . . -178.1(6) no
C3 C4 C5 C10 . . -177.6(6) no
C9 C4 C5 C10 . . 3.0(10) no
C4 C5 C6 C1 . . 1.0(10) no
C10 C5 C6 C1 . . -179.7(6) no
C2 C1 C6 C5 . . -2.0(10) no
C7 C1 C6 C5 . . 178.8(6) no
Zn3 O1 C7 O2 4_576 . 28.0(10) no
Zn3 O1 C7 C1 4_576 . -146.2(5) no
Zn2 O2 C7 O1 2_556 . -7.0(10) no
Zn2 O2 C7 C1 2_556 . 166.6(4) no
C2 C1 C7 O1 . . -73.7(9) no
C6 C1 C7 O1 . . 105.5(7) no
C2 C1 C7 O2 . . 111.6(7) no
C6 C1 C7 O2 . . -69.1(8) no
Zn1 O4 C8 O3 2_656 . -5.0(10) no
Zn1 O4 C8 C2 2_656 . 174.9(4) no
Zn3 O3 C8 O4 4_676 . 3.0(10) no
Zn3 O3 C8 C2 4_676 . -177.1(5) no
C1 C2 C8 O4 . . -19.0(10) no
C3 C2 C8 O4 . . 158.7(6) no
C1 C2 C8 O3 . . 161.0(6) no
C3 C2 C8 O3 . . -21.3(9) no
Zn3 O5 C9 O6 . . 166.4(5) no
Zn3 O5 C9 C4 . . -18.6(9) no
Zn2 O6 C9 O5 1_655 . 0.5(7) no
Zn2 O6 C9 C4 1_655 . -174.7(4) no
C3 C4 C9 O5 . . -118.8(7) no
C5 C4 C9 O5 . . 61.1(9) no
C3 C4 C9 O6 . . 56.3(8) no
C5 C4 C9 O6 . . -123.7(7) no
Zn1 O8 C10 O7 . . -7.0(10) no
Zn3 O8 C10 O7 . . 176.9(5) no
Zn1 O8 C10 C5 . . 174.6(4) no
Zn3 O8 C10 C5 . . -1.5(9) no
Zn2 O7 C10 O8 . . 6.0(10) no
Zn2 O7 C10 C5 . . -175.7(5) no
C6 C5 C10 O8 . . 129.7(7) no
C4 C5 C10 O8 . . -50.9(9) no
C6 C5 C10 O7 . . -48.9(9) no
C4 C5 C10 O7 . . 130.5(7) no
